Earth Shield® Type 10 Mastic Waterstop is certified for use in Federal Specification SS-S-210A.
July 2, 1975
Int. Fed. Spec. SS-S-00210 (GSA-FSS)
July 26, 1965
SEALING COMPOUND, PREFORMED PLASTIC, FOR EXPANSION JOINTS AND PIPE JOINTS
This specification was approved by the Commissioner, Federal Supply
Service, General Services Administration, for the use of all Federal
1. SCOPE AND CLASSIFICATION
1.1 Scope. This specification covers a cold-applied preformed plastic
sealing compound or sealing expansion joints and tongue and groove joints of
concrete pipe culvert, storm drain and sewer pipe.
1.2 Classification. The sealing compound shall be of one grade and of
the following types and sizes, as specified (see 6.2).
Type I - Rope Form.
Sizes Diameter Length
1/2" 2' 6"
3/4" 2' 0"
3/4" 2' 6'
1" 2' 6"
1 1/2" 2' 6"
1 1/2" 3' 8"
1 3/4" 3' 8"
2" 3' 8"
Type II - Flat Tape Form.
Sizes Thickness Width
1/8" 1 1/2"
3/16" 1 1/2"
1/4" 1 1/2"
(Lengths of flat tapes shall be 2'6", 3'8', and 4'0" for all foregoing
2. APPLICABLE DOCUMENTS
2.1 The following documents, of the issues in effect on date of
invitation for bids or request for proposal, form a part of this
specification to the extent specified herein.
PPP-B-636 - Boxes, Shipping, Fiberboard.
Fed. Test Method Std. No. 141 - Paint, Varnish, Lacquer, and Related
Materials; Methods of Inspection,
Sampling and Testing.
Int. Fed. Test Method Std. No. 210 - Road and Paving Materials, Methods
of Sampling and Testing.
Fed. Std. No. 102 - Preservation, Packaging, and Packing Levels.
Fed. Std. No. 123 - Marking for Shipment (Civil Agencies).
(Activities outside the Federal Government may obtain copies of Federal
Specifications, Standards, and Handbooks as outlined under General
Information in the Index of Federal Specifications and Standards and at the
prices indicated in the Index. The Index, which includes cumulative monthly
supplements as issued, is for sale on a subscription basis by the
Superintendent of Documents, U.S. Government Printing Office, Washington, DC
(Single copies of this specification and other Federal Specifications
required by activities outside the Federal Government for bidding purposes
are available without charge from Business Service Centers at the General
Services Administration Regional Offices in Boston, New York, Washington, DC,
Atlanta, Chicago, Kansas City, MO, Fort Worth, Denver, San Francisco, Los
Angeles, and Seattle, WA.)
(Federal Government activities may obtain copies of Federal
Specifications, Standards, and Handbooks and the Index of Federal
Specifications and Standards from established distribution points in their
MIL-STD-129 - Marking for Shipment and Storage.
MIL-STD-105 - Sampling Procedures and Tables for Inspection by
(Copies of Military Specifications and Standards required by suppliers in
connection with specific procurement functions should be obtained from the
procuring activity or as directed by the contracting officer.)
2.2 Other publications. The following documents form a part of this
specification to the extent specified herein. Unless a specific issue is
identified, the issue in effect on date of invitation for bids or request for
proposal shall apply.
American Society for Testing and Materials (ASTM) Publications:
D4 - Bitumen.
D6 - Loss on Heating of Oil and Asphaltic Compounds.
D36 - Softening Point of Asphalts and Tar Pitches.
D71 - Specific Gravity of Solid Pitch and Asphalt.
D92 - Flash and Fire Points by Cleveland Open Cup.
D113 - Ductility of Bituminous Materials.
D217 - Cone Penetration of Lubricating Grease.
(Application for copies should be addressed to the American Society for
Testing and Materials, 1916 Race Street, Philadelphia, PA 19103.)
National Motor Freight Traffic Association, Inc., Agent:
National Motor Freight Classification.
(Application for copies should be addressed to the American Trucking
Associations, Inc., Tariff Order Section, 1616 P Street, N.W., Washington, DC
Uniform Classification Committee, Agent:
Uniform Freight Classification.
(Application for copies should be addressed to the Uniform Classification
Committee, Room 1106, 222 South Riverside Plaza, Chicago, IL 60606.)
3.1 Description. The sealing compound furnished under this
specification shall be produced from blends of refined hydrocarbon resins
and plasticizing compounds reinforced with inert mineral filler, and shall
contain no solvents, irritating fumes or obnoxious odors. The compound shall
not depend on oxidizing, evaporating, or chemical action for its adhesive or
cohesive strength. It shall be supplied in either extruded rope-form of
suitable cross-section or flat tape form and of such sizes as to fill the
joint space when the pipes are laid.
3.2 Chemical Composition. The chemical composition of the sealing
compound shall meet the requirements shown in Table I when tested as
specified in 4.5.
Components Minimum Maximum
Bitumen % by weight 50 70
Inert Mineral Filler % by weight 30 50
Volatile Matter % by weight -- 2.0
3.3 Physical properties The physical properties of the sealing compound
shall meet the requirements shown in Table II when tested as specified in
Specific Gravity @ 77 deg. F. (25 deg. C.) 1.20 to 1.35
Ductility @ 77 deg. F. (25 deg. C.) Min. 5.0 cm
Softening Point @ 77 deg. F. Min. 320 deg. F.
Flash Point, C.O.C. Min. 600 deg. F.
Fire Point, C.O.C. Min. 625 deg. F.
77 deg. F. (25 deg. C.) (150 gs.) 5 sec. 50 to 120
3.4 Adhesion and hydrostatic pressure. The sealing compound shall not
leak at the joints for a period of 24 hours when tested as specified in
3.5 Sag or flow resistance (vertical or overhead joint). No sagging
shall be detected when tested as specified in 4.5.3.
3.6 Chemical resistance. The sealing compound when immersed separately
in a 5 percent solution of caustic potash, a 5 percent solution of
hydrochloric acid, a 5 percent solution of sulfuric acid and a saturated hydrogen sulfide solution for 30 days at ambient room temperature shall show
no visible deterioration.
3.7 Workmanship. Workmanship shall be in accordance with good
commercial practice for this type of commodity.
4. QUALITY ASSURANCE PROVISIONS
4.1 Responsibility for inspection. Unless otherwise specified in the
contract or purchase order, the supplier is responsible for the performance
of all inspection requirements as specified herein. Except as otherwise
specified in the contract or order, the supplier may use his own or any other
facilities suitable for the performance of the inspection requirements
specified herein, unless disapproved by the Government. The Government
reserves the right to perform any of the inspections set forth in the
specification where such inspections are deemed necessary to assure that
supplies and services conform to prescribed requirements.
4.2 Sampling. Sampling shall be performed in accordance with Methods
101.11 and 101.21 of Interim Federal Test Method Standard No. 210 Road and
4.3 Inspection. Inspection shall be performed in accordance with Method
1011 of Federal Test Method Standard No. 141.
4.4 Inspection of preparation for delivery requirements. An inspection
shall be made to determine that the packing and marking comply with the
requirements in section 5 of this specification. Defects shall be scored in
accordance with Table III. The sample unit shall be one shipping container
fully prepared for delivery. Sampling shall be in accordance with
MIL-STD-105. The lot size shall be the number of shipping containers in the
end item inspection lot. The inspection level shall be II with an acceptable
quality level (AQL) of 4.0 defects per hundred units.
TABLE III. Classification of preparation for delivery defects
Markings (exterior and interior) Omitted; incorrect; illegible; improper
size, location, sequence, or method of
Materials Any component missing, or damaged.
Workmanship Inadequate application of components such
as incomplete closure of container flaps,
loose strapping, inadequate stapling.
Distortion of container.
4.5.1 The following tests shall be made in accordance with the methods
shown in Table IV and as described hereinafter. Each test shall be run in
triplicate and if more than one specimen fails the test, the lot represented
by that specimen shall be rejected.
TABLE IV. Test methods
Bitumen ASTM D4
Inert Mineral Filler Int. Fed. Test Method Std. No. 210
Volatile Matter ASTM D6
Specific Gravity ASTM D71
Ductility ASTM D113
Softening Point ASTM D36
Flash Point ASTM D92
Fire Point ASTM D92
Cone Penetration ASTM D217
4.5.2 Adhesion and hydrostatic pressure. Mount a vertical column using
2 1/2 sections of 3 foot 6 inch bell and spigot or tongue and groove pipe.
Seal the 1/2 section to a concrete slab with the sealing compound and follow
with the other two sections. Immediately fill the pipe sections with water
to obtain an approximate 6 foot head pressure. Mount a horizontal column
using 3 sections of 12 inch to 36 inch tongue and groove pipe and apply the
sealing compound to seal the tongue and groove joints, the metal end plates,
bolts and washers. Draw multiple pipe section together until a 1/8 inch to
3/16 inch squeeze-out is observed at all joints. Immediately fill pipes
with water, slowly applying hydrostatic pressure in increments of 2 pounds
per square inch every minute until 10 psi is reached.
4.5.3 Sag or flow resistance (vertical or overhead joints). Fill a
wooden form 1 inch wide and 6 inches long flush with sealing compound and
place in an oven at 135 deg. F, in a vertical position for 5 days.
5. PREPARATION FOR DELIVERY
5.1 Packing. Packing shall be level A, B or C as specified.
5.1.1 Level A. The compound of like description furnished in sizes,
lengths and quantities as specified (see 6.2) shall be packed in a
close-fitting box conforming to PPP-B-636, class weather resistant. The box
shall be closed and strapped in accordance with the appendix to the box
5.1.2 Level B The compound shall be packed in accordance with 5.1.1,
except the fiberboard box shall be class domestic and the closure shall be
in accordance with method II of PPP-B-636.
5.1.3 Level C. The compound shall be packed to insure carrier
acceptance and safe delivery at destination in containers complying with the
National Motor Freight Classification rules or the Uniform Freight
5.2.1 Civil agencies. In addition to markings required by the contract
or order, the shipping containers shall be marked in accordance with Fed.
Std. No. 123.
5.2.2 Military activities. In addition to markings required by the
contract or order, the shipping containers shall be marked in accordance
6.1 Intended use The cold-applied preformed plastic sealing compound
covered by this specification is intended for sealing expansion joints and
tongue and groove concrete pipe.
6.2 Ordering data. Purchasers should select the preferred options
permitted herein, and include the following information in procurement
(a) Title, number, and date of this specification.
(b) Lengths, sizes and quantities of compound required (see 1.2).
(c) Level of packing required (see 5.1).
(d) whether civil or military marking is required (see 5.2).
Orders for this publication are to be placed with General Services
Administration, acting as an agent for the Superintendent of Documents. See
Section 2 of this specification to obtain extra copies and other documents
December 16, 1981
October 31, 1978
SEALING COMPOUND, PREFORMED PLASTIC,
FOR EXPANSION JOINTS AND PIPE JOINTS
This notice as approved by the Commissioner, Federal Supply Service,
General Services Administration.
This notice is issued to reinstate Federal Specification SS-S-210A,
dated July 2, 1975.
Cancellation notice dated October 31, 1978, is hereby canceled.